Dear Label_Name,

Greetings! I hope you are well.

I am writing on behalf of an international publishing house, Science and Education Publishing, USA (http://www.sciepub.com).

Science and Education Publishing (SciEP) is a multidisciplinary open access publisher of Journals covering the fields of Science, Technology and Medicine. All SciEP publications are subject to high-quality peer review, editorial and production processes and are freely available online.

Welcome to the April, 2013 edition of SciEP newsletter, providing monthly summaries of articles on science & education related topics of interest to scientist and professionals. The mission of our journals is to provide an open access forum for publishing new findings on issues pertinent to scientific and academic field. We also invite you to submit original research papers, review articles, short reports, or case studies are considered for publication in our Multidisciplinary Journals.

American Journal of Public Health Research
DOI: 10.12691/ajphr-1-1-3

The Implementation of a Tele-Homecare System with Service Oriented Architecture and HL7 Message Transmission Standard
Ching-Sung Wang

American Journal of Medical and Biological Research
DOI: 10.12691/ajmbr-1-1-2

The Influence of Ethanol on Pyruvate Kinases Activity in Vivo, in Vitro, in Silico
Lelevich Sergey Vladimirovich, Khrustalev Vladislav Victorovich, Barkovsky Eugene Victorovich, Shedogubova Tatyana Aleksandrovna

American Journal of Medical Sciences and Medicine
DOI: 10.12691/ajmsm-1-1-1

Clinical and Histological Features in Wegener Granulomatosis
Li Cavoli Gioacchino, Passantino Rita, Bono Luisa, Tortorici Calogera, Ferrantelli Angelo, Giammarresi Carlo, Rotolo Ugo

American Journal of Infectious Diseases and Microbiology
DOI: 10.12691/ajidm-1-1-2

The Curse of Lymphatic Filariasis: Would the Continual Use of Diethylcarbamazine Eliminate this Scourge in Papua New Guinea?
Anne Lanham, Lillian Mwanri

We have released issues of some journals on February 2013.
American Journal of Public Health Research
American Journal of Medical Sciences and Medicine
American Journal of Medical and Biological Research
American Journal of Pharmacological Sciences
American Journal of Clinical Medicine Research
American Journal of Nursing Research
American Journal of Cancer Prevention
American Journal of Medicine Studies
American Journal of Infectious Diseases and Microbiology
American Journal of Cardiovascular Disease Research
American Journal of Biomedical Research
American Journal of Mechanical Engineering
American Journal of Microbiological Research
Journal of Preventive Medicine
American Journal of Food and Nutrition
American Journal of Hypertension Research
American Journal of Sports Science and Medicine
Journal of Cancer Research and Treatment
American Journal of Zoological Research
Journal of Biomedical Engineering and Technology
American Journal of Microbiological Research
Biomedical Science and Engineering

We are pleased to announce that submissions are now being accepted for peer review for all the journals across all our subject areas in SciEP.

Please submit your manuscript via our online submission system:
http://www.sciepub.com/author/signin

To unsubscribe from our mailing list, please click on the following link: unsubscribe

I am looking forward to hearing from you.

Kind regards,

David Rain
Email:join@sciepub.com
Science and Education Publishing (http://www.sciepub.com)

Elastic and Acoustic Properties of XB₂ (X= V, Nb & Ta) Transition Metal Diborides

Pramod Kumar Yadawa

Department of Applied Physics, AMITY School of Engineering and Technology, New Delhi- 110 061, India

Abstract: The elastic properties, acoustic properties and mechanical properties of the group VB transition metal diborides like VB₂, NbB₂ and TaB₂ have been studied along unique axis at room temperature. The second- and third order elastic constants (SOEC & TOEC) have been calculated for these diborides using Lennard–Jones potential model. The velocities VL and VS2 increases with the angle from the unique axis and VS1 have maximum at 45° with unique axis of the crystal. The inconsistent behaviour of angle dependent velocities is associated to the action of second order elastic constants. Debye average sound velocities of these compounds are increasing with the angle and has maximum at 55° with unique axis at room temperature. Hence when a sound wave travels at 55° with unique axis of these materials, then the average sound velocity is found to be maximum. The mechanical properties of VB₂ are better than TaB₂, because VB₂ has low ultrasonic attenuation comparison than TaB₂. The diborides are good electrical conductors; they are attractive for the same types of applications as other hard refractory materials such as in composite and in hard coating. Traditional applications o such materials are based on their interesting combination of mechanical and transport properties.

Keywords: elastic properties, VB transition metal diborides, thermal conductivity, acoustic properties

Received April 29, 2015; Revised May 11, 2015; Accepted May 19, 2015

Citation: Pramod Kumar Yadawa, Elastic and Acoustic Properties of XB₂ (X= V, Nb & Ta) Transition Metal Diborides. Journal of Materials Physics and Chemistry, 3 (1). 1-5. January 2015. doi:10.12691/jmpc-3-1-1

1. Introduction

VB transition metal diborides are interest for fundamental reasons as well as for practical applications. Borides of transition metals have various unique properties which in many cases are of great importance from technological view points. Among their attractive properties are high thermal and chemical stability, high electrical and thermal conductivity, and high hardness and high mechanical stiffness [1]. VB transition metal diborides XB₂ (X= V, Nb and Ta) with the hexagonal structure have attracted much attention because of its physical and chemical properties such as wear resistance, corrosion resistance, high hardness, high melting point and oxidation, and extensive industrial applications [2,3,4,5,6].

Ultrasonics techniques are widely used for the determination of elastic properties and the characterization of the microstructure of materials. The elastic constants are determined by the measurement of velocities of the longitudinal and shear waves [7], while the microstructure is generally evaluated by measuring their attenuation [8]. Ultrasonic also offers the possibility of measuring texture [9,10], phase change and residual stresses [11]. Ultrasonic velocity and attenuation has been shown also to correlate in certain cases to fracture toughness and fatigue damage [12]. Recently ultrasonic velocity and attenuation has been studied in various physical states and conditions.

There are three types of acoustic mode lattice vibration: one longitudinal acoustic and two transverse acoustical for hexagonal and cubic structured materials [13,14]. Hence, there are three types of acoustic wave velocities for each direction of propagation of wave, which are well related to second order elastic constants. But all the three type of orientation dependent acoustic wave velocity of these all materials are not reported in literature. Therefore in this paper, we predict the ultrasonic properties of hexagonal structured VB₂, NbB₂ and TaB₂ at room temperature. The ultrasonic attenuation coefficient, acoustic coupling constants, higher order elastic constants, thermal relaxation time and ultrasonic wave velocities for these diborides for each direction of propagation of wave are calculated at room temperature. The calculated ultrasonic parameters are discussed with related thermophysical properties for the characterization of the chosen compounds. The obtained results are interesting for characterization of these diborides materials.

2. Theory

In the present investigation, the theory is divided into two parts:

2.1. Second and Third Order Elastic Constants

The second (CIJ) and third (CIJK) order elastic constants of material are defined by following expressions.

[picture] | (1)

[picture] | (2)

where, U is elastic energy density, eI=eij (i or j = x, y, z, I=1, …6) is component of strain tensor. Equations (1) and (2) leads six second and ten third order elastic constants (SOEC and TOEC) for the hexagonal close packed structure materials [15,16].

[picture] | (3a)

[picture] | (3b)

where p = c/a: axial ratio;; ; ; m, n=integer quantity; b₀=Lennard Jones parameter.

2.2. Ultrasonic Attenuation and Allied Parameters

The predominant causes for the ultrasonic attenuation in a solid at room temperature are phonon-phonon interaction (Akhieser loss) and thermoelastic relaxation mechanisms. The ultrasonic attenuation coefficient (A)Akh due to phonon-phonon interaction and thermoelastic relaxation mechanisms is given by the following expression [17,18].

[picture] | (4)

[picture] | (5)

where, f: frequency of the ultrasonic wave; ρ :the density of the material V: ultrasonic velocity for longitudinal and shear wave; VL: longitudinal ultrasonic velocity; E₀: thermal energy density; : Grüneisen number (i, j are the mode and direction of propagation).

The Grüneisen number for hexagonal structured crystal along <001> orientation or θ=0⁰ is direct consequence of second and third order elastic constants. is known as acoustic coupling constant, which is the measure of acoustic energy converted to thermal energy. When the ultrasonic wave propagates through crystalline material, the equilibrium of phonon distribution is disturbed. The time for re-establishment of equilibrium of the thermal phonon distribution is called thermal relaxation time (τ) and is given by following expression:

[picture] | (6)

Here τL and τS are the thermal relaxation time for longitudinal and shear wave. ‘k’ and CDYV are the thermal conductivity and specific heat per unit volume of the material respectively. The Debye average velocity (VD) is well related to longitudinal (VL) and shear wave (VS1, VS2) velocities. The expressions for ultrasonic velocities are given in our previous paper [16].

3. Results & Discussion

3.1. Higher Order Elastic Constants

The unit cell parameters ‘a’ (basal plane parameter) and ‘p’ (axial ratio) for VB₂, NbB₂ and TaB₂ are 2.993Å, 3.107Å, 3.104Å and 1.012, 1.067, 1.133 respectively [19]. The value of m and n for chosen materials are 6 and 7. The values of b₀ are 2.5x10⁻⁶⁴ erg cm⁷, 4.0x10⁻⁶⁴ and 3.0x10⁻⁶⁴ erg cm⁷ for VB₂, NbB₂ and TaB₂ respectively. The SOEC and TOEC have been calculated for these compounds using equation. (3) and bulk modulus (B) are presented in Table 1.

Table 1. Second and third order elastic constants (SOEC and TOEC) & Bulk Modulus (B) in the unit of GPa of VB₂, NbB₂ and TaB₂ compounds at room temperature

The elastic constants of the material are important, since they are related to hardness and therefore of interest in applications where mechanical strength and durability are important. Also, the second order elastic constants are used for the determination of the ultrasonic attenuation and related parameters. It is obvious from Table 1 that, there is good agreement between the present and reported theoretical and experimental second order elastic constants and bulk modulus of VB₂, NbB₂ and TaB₂ [19]. The bulk modulus (B) for these compounds can be calculated with the formula B= 2(C₁₁+ C₁₂+ 2C₁₃ + C₃₃/2)/9 [20]. Hence applied theory for the evaluation of higher order elastic constants at room temperature is justified.

3.2. Ultrasonic Velocity and Allied Parameters

The density and thermal conductivity at room temperature have been taken from the previous works [21,22,23]. The value of CV and E₀ are evaluated using tables of physical constants and Debye temperature. The quantities ρ, CV and E₀, ‘k’ and calculated acoustic coupling constants (DL and DS) are presented in Table 2.

Table 2. Density (ρ: in 10³ kg m⁻³), specific heat per unit volume (CV: in 10⁶ Jm⁻³ K⁻¹ ), thermal energy density (E₀: in 10⁸ Jm⁻³ ), thermal conductivity (k: in Wm⁻¹ K⁻¹) and acoustic coupling constant (DL, DS) of VB₂, NbB₂ and TaB₂ compounds

The calculated orientation dependent ultrasonic wave velocities and Debye average velocities at room temperature are shown in Figure 1–Figure 4. Figure 1–Figure 3 show that the VL and VS2 increases with the angle from the unique axis and VS1 have maximum at 45⁰ with unique axis of the crystal. The combined effect of SOEC and density is cause for abnormal behaviour of angle dependent velocities.

Figure 1. VL vs angle with unique axis of crystal

Figure 2. VS1 vs angle with unique axis of crystal

The nature of the angle dependent velocity curves in the present work is found similar as that for other hexagonal diborides materials [20,24]. Thus the computed velocities for these materials are justified.

Debye average velocities (VD) of these compounds are increasing with the angle and have maxima at 55° at 300 K (Figure 4). Since VD is calculated using VL, VS1 and VS2 [24], therefore the angle variation of VD is influenced by the constituent ultrasonic velocities. The maximum VD at 55° is due to a significant increase in longitudinal and pure shear (VS2) wave velocities and a decrease in quasi-shear (VS1) wave velocity. Thus it can be concluded that when a sound wave travels at 55° with the unique axis of these materials then the average sound wave velocity is maximum.

Figure 3. VS2 vs angle with unique axis of crystal

Figure 4. VD vs angle with unique axis of crystal

The thermal relaxation time for hexagonal structured material follows the equation τ= τo exp (x/λ), where ‘τ’ and ‘λ’ are constants. The order of ‘τ’ for hexagonal structure diborides is in picoseconds [20]. With reference some previous work [25,26], the size dependency of ‘τ’ for bcc and fcc structured materials follow the equation τ= τo [1- exp (-x/λ)]. Thus it can be said that the thermal relaxation time is not only function of size and temperature but also depends on the structure of a materials. Hence the calculated τ justifies the hexagonal structure of chosen compounds at room temperature. The minimum ‘τ’ for wave propagation along θ = 55⁰ implies that the re-establishment time for the equilibrium distribution of thermal phonons will be minimum for propagation of wave along this direction.

Figure 5. Relaxation time vs angle with unique axis of crystal

Thus the present average sound velocity directly correlates with the Debye temperature, specific heat and thermal energy density of these materials.

3.3. Ultrasonic Attenuation

In the evaluation of ultrasonic attenuation, it is supposed that wave is propagating along the unique axis (<001> direction) of these metals. The attenuation coefficient over frequency square (A/f²)Akh for longitudinal (A/f²)L and shear wave (A/f²)S are calculated using Equation (4) under the condition ωτ<<1 at room temperature. Thermoelastic loss over frequency square (A/f²)Th is calculated with the Equation (5). The values of (A/f²)L, (A/f²)S, (A/f²)Th. and total attenuation (A/f²)Total are presented in Table 3.

Table 3. Ultrasonic attenuation coefficient (in 10⁻¹⁸ Nps²m⁻¹) of VB₂, NbB₂ and TaB₂ compounds

In the present investigation, the ultrasonic wave propagates along the unique axis of the crystal, the Akhieser type of loss of energy for longitudinal and shear wave and thermo elastic loss increases with the temperature of the material (Table 3). (A/f²)Akh is proportional to D, E₀, τ and V⁻³ (Equations. 4 and 6). The E₀ is increasing and V is decreasing with the temperature (Figure 1-Figure 3). Hence, Akhieser loss in these compounds is predominantly affected by the thermal energy density E₀ and the thermal conductivity.

Therefore, the ultrasonic attenuation increases due to the reduction in the thermal conductivity. Thus ultrasonic attenuation is mainly governed by the phonon–phonon interaction mechanism. A comparison of the ultrasonic attenuation could not be made due to lack of experimental data in the literature.

Table 3 indicate that the thermoelastic loss is very small in comparison to Akhieser loss and ultrasonic attenuation for longitudinal wave (A/f²)L is greater than that of shear wave (A/f²)S. This reveals that ultrasonic attenuation due to phonon-phonon interaction along longitudinal wave is governing factor for total attenuation ((A/f²)Total =(A/f²)Th+(A/f²)L+(A/f²)S). The total attenuation is mainly affected by thermal energy density and thermal conductivity. Thus it may predict that at room temperature VB₂ behaves as its purest form and is more ductile as evinced by minimum attenuation comparison than TaB₂.

Since ultrasonic attenuation (A) ∝ V⁻³ and ultrasonic velocity is the largest for VB₂ compound among TaB₂ compound thus the attenuation (A) have smallest for VB₂ and material should be most ductile. The minimum ultrasonic attenuation for VB₂ justifies its quite stable hexagonal structure state. The attenuation of these diborides is smaller than other diborides compounds (TiB₂, MnB₂, TcB₂, ReB₂ and OsB₂) due to their smaller velocities [20,24,27]. This implies that the interaction between acoustical phonon and quanta of lattice vibration for these VB transition metal diborides is smaller in comparison to other group diborides.

4. Conclusions

Present method to evaluate second and third order elastic constants involving much body interaction potential for hexagonal structured VB transition metal diborides compounds is correct. All elastic constants and density are mainly the affecting factor for anomalous behaviour of ultrasonic velocity in these compounds. The order of thermal relaxation time for these compounds is found in picoseconds, which justifies their hexagonal structure. The re-establishment time for the equilibrium distribution of thermal phonons will be minimum for the wave propagation along θ = 55⁰ due to being smallest value of τ along this direction. The acoustic coupling constant of these group compounds for longitudinal wave are found larger than other group diborides. Hence the conversion of acoustic energy into thermal energy will be large for these compounds. The ultrasonic attenuation due to phonon-phonon interaction mechanism is predominant over total attenuation as a governing factor thermal conductivity.

The mechanical properties (yield strength, ductility, elastic properties) of VB₂ are better than TaB₂, because at VB₂ has high ultrasonic velocity and low ultrasonic attenuation. The results obtain in this investigation can be used for further study of these transition metal diborides. Our whole theoretical approach can be applied to the evaluation of ultrasonic attenuation and related parameters to study the michrostructural properties of hexagonal structured materials.

References

[1]   | Aronsson, B., Rundqvist, S. and Lundstrom, T., “Borides, silicides and phosphides”, Methuen, London: 1. 1965.
[2]   | Varin, R A., Chiu, C., Li, S., Calka A. and Wexler, D., “Application of controlled and electrical discharge assisted mechanical alloying for the synthesis of nano crystalline MgB₂ superconducting compound”, J. Alloys Compd. 370. 230-243. 2004.
[3]   | Erdemir, A., Halter, M. and Fenske, G. R.,“Preparation of ultralow-friction surface films onvanadium diboride”, Wear 205. 236-239. 1997.
[4]   | ] Shein, I.R. and Ivanovskii, A. L., “Influence of lattice vacancieson the structural, electronic and cohesive properties of niobiumand molybdenum borides from first-principles calculations”, Phys.Rev.B73. 144108-144116. 2006.
[5]   | Deligoz, E., Colakoglu, K. and Ciftci, Y. O., “Lattice dynamical properties of ScB₂, TiB₂ and VB₂ compounds”, Solid State Commun.149. 1843-1848. 2009.
[6]   | Zhou, W., Wu, H. and Yildirim, T. “Electronic, dynamical, and thermal properties of ultra-in compressible superhard rhenium diboride: a combined first- principles and neutron scattering study”, Phys. Rev. B 76. 184113-184118. 2007.
[7]   | Landa, M., Novak, V., Sedlak, P. and Sittner, P., “Ultrasonic characterization of Cu-Al-Ni single crystals lattice stability in the vicinity of the phase transition”, Ultrasonics, 42. 519-526. 2004.
[8]   | Levelut, C., Le parc R. and Pelous, J., “Dynamic sound attenuation at hypersonic frequencies in silica glass”, Phys. Rev. B 73. 052202. (1-3). 2006.
[9]   | Wu, J., Layman, C., Murthy, S. and Ruey-Bin Yang, “Determine mechanical properties of particulate composite using ultrasound spectroscopy”, Ultrasonics, 44. 793-800. 2006.
[10]   | Hukong and Zhu, C., “Origin of cracking in nanoscale Cu/Ta multilayers”, Appl. Phys. Letters 88. 041920 (1-3). 2006.
[11]   | Allen, D. R., Copper, W. H. B., Sayer, C. M. and Silk, M. G., “Research techniques in non-destructive testing”, R. S. Sharpe (Ed), Vol. 6 151-209 Academic Press, New York, 1982.
[12]   | Gudkov, V., Lonchakov, A., Sokolov, V., Zhevstovskikh, I. and Gruzdev, N., Phys. Stat. Sol. (B) 242 (3) R30-R32. 2005.
[13]   | Rosen, M. and Klimker, H. “Low-Temperature Elasticity and Magneto-Elasticity of Dysprosium Single Crystals”, Phys. Rev. B 1. 3748. 1970.
[14]   | Alers, G. A. and Neighbours, J. R., “The elastic constants of zinc between 4.2° and 670°K”, J. Phys. Chem. Solids, 7. 58. 1958.
[15]   | Yadawa, P. K. “Acoustic wave propagation in Ni₃R (R= Mo, Nb, Ta) compounds”, Pramana, 76(4). 613-619. 2011.
[16]   | Yadawa, P. K. “Behaviour of ultrasonic velocities and elastic constants in Ag-Zn alloys”, Advanced Material Letters, 2(2). 157-162. 2011.
[17]   | Pandey, D. K., Yadawa, P. K. and Yadav, R. R., “Ultrasonic properties of hexagonal ZnS at nanoscale,” Mat. Lett., 61. 5194-5198. 2007.
[18]   | Pandey, D. K., Yadawa, P. K. and Yadav, R. R. “Acoustic wave propagation in laves phase compounds,” Mat. Lett., 61. 4747-4751. 2007.
[19]   | Qi, C. J., Jiang, Y. H., Liu, Y. Z. and Zhou, “Elastic and electronic properties of Xb₂ (X= V, Nb, Ta, Cr, Mo and W) with AlB₂ structure from first principles calculations”, Ceramics Interational, 40.5843-5851. 2014.
[20]   | Yadawa, P. K., “Elstic and acoustic properties of hexagonal MnB₂, TcB₂ and ReB₂ compounds”, Journal of Advanced Physics, 2. 111-115. 2013.
[21]   | Shein, I. R. and Lvanovskii, A. L., “Band structure of ZrB₂, VB₂, NbB₂, and TaB₂ hexagonal diborides: Comparison with superconducting MgB₂”, Phys. Solid State 44. 1833. 2002.
[22]   | Islam, A. K. M. A., Sikder, A. S. and Islam, F. N., “NbB₂ : A density functional study”, Physics Letters A 350. 288-292. 2006.
[23]   | Zhao, W. J. and Wang, Y. X., “Structural, mechanical and electronic properties of TaB₂, TaB, IrB₂, IrB : First principle calculations”, Journal of Solid State Chemistry, 182. 2880-2886. 2009.
[24]   | Yadawa, P. K., “Ultrasonic characterization of ceramic material titanium diboride”, Ceramics-Silikaty. 55(2). 127-133. 2011.
[25]   | Yadav, R. R. and Pandey, D. K., “Ultrasonic properties at the nanoscale in some metals”, Materials Letters, 59. 564. 2005.
[26]   | Yadav, R. R. and Pandey, D. K., “Size dependent acoustical properties of bcc metals”, Acta Phys. Polonica A, 107. 933. 2005.
[27]   | Yadawa, P. K., “Ultrasonic Characterization of Superhard Material: Osmium Diboride”, IOP Conf. Series: Material Science and Engineering, 42. 012034. 2012.